Syntheses, Crystal Structures, and Luminescent Properties of Novel Layered Lanthanide Sulfonate-Phosphonates
Jun-Ling Song; Chong Lei; Jiang-Gao Mao; Inorganic Chemistry 43 (2004) 5630–5634; doi:10.1021/ic049376u

data_4311481
_publ_contact_author_address
;
     Fujian Institute of Research  
        on the Structure of Matter,
        Chinese Academy of Sciences,
        Fuzhou, Fujian 350002, 
    P.R.China
;
_publ_contact_author_email       mjg@ms.fjirsm.ac.cn
_publ_contact_author_fax         0086-0591-3714946
_publ_contact_author_name        'Dr. Jiang-Gao Mao'
_publ_contact_author_phone       0086-0591-3704836
_publ_section_title
;
 Syntheses, Crystal Structures, and Luminescent Properties of Novel
 Layered Lanthanide Sulfonate-Phosphonates
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5630
_journal_page_last               5634
_journal_paper_doi               10.1021/ic049376u
_journal_volume                  43
_journal_year                    2004
_chemical_formula_moiety         'C12 H19 N O15 P Pr S'
_chemical_formula_sum            'C12 H19 N O15 P Pr S'
_chemical_formula_weight         621.22
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                73.3390(10)
_cell_angle_beta                 81.2610(10)
_cell_angle_gamma                77.0600(10)
_cell_formula_units_Z            2
_cell_length_a                   7.66690(10)
_cell_length_b                   11.4004(2)
_cell_length_c                   12.012
_cell_measurement_temperature    293(2)
_cell_volume                     975.96(2)
_computing_cell_refinement       'Smart CCD Software(Siemens, 1994)'
_computing_data_collection       'Smart CCD Software(Siemens, 1994)'
_computing_data_reduction        'Smart CCD Software(Siemens, 1994)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Smart CCD'
_diffrn_measurement_method       '\w scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0649
_diffrn_reflns_av_sigmaI/netI    0.0563
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            5117
_diffrn_reflns_theta_full        25.08
_diffrn_reflns_theta_max         25.08
_diffrn_reflns_theta_min         1.78
_diffrn_standards_decay_%        0.9
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  .
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.766
_exptl_absorpt_correction_T_max  0.9776
_exptl_absorpt_correction_T_min  0.4889
_exptl_absorpt_correction_type   PSI
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.114
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       brick
_exptl_crystal_F_000             616
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_refine_diff_density_max         1.867
_refine_diff_density_min         -2.306
_refine_diff_density_rms         0.225
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.114
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     280
_refine_ls_number_reflns         3422
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.114
_refine_ls_R_factor_all          0.0652
_refine_ls_R_factor_gt           0.0565
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0436P)^2^+17.8581P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1335
_refine_ls_wR_factor_ref         0.1421
_reflns_number_gt                3094
_reflns_number_total             3422
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic049376usi20040513_120519.cif
_cod_data_source_block           psi
_cod_original_cell_volume        975.92(2)
_cod_database_code               4311481